# analytical methods for materials - weaver research group analytical methods for materials laboratory

Post on 14-Jun-2020

1 views

Category:

## Documents

Embed Size (px)

TRANSCRIPT

• Analytical Methods for Materials

Laboratory Module #4 Phase Diagram Determination

Suggested Reading • C. Suryanarayana and M.G. Norton, X-ray Diffraction A Practical Approach, (Plenum Press, New York,

1998), pages 167-192. • B.D. Cullity and S.R. Stock, Elements of X-ray Diffraction, 3rd Edition, (Prentice-Hall, Upper Saddle

River, NJ, 2001), Ch. 11, pages 331-346. • F.N. Rhines, Phase Diagrams In Metallurgy, (McGraw-Hill, New York, NY, 1956).

708

• Objectives

• Upon completion of this module you will be able to use the lattice parameter determination techniques to determine the solid solubility of one element/compound into another and to construct experimental phase diagrams.

709

• Background

• Phase diagrams: – Used to establish what phases are present at

different temperatures, pressures and compositions within an alloy system.

• Maps of phases that are present under specific conditions.

• Pressure – Temperature – Composition – P-T-x diagrams

710

• 711

A B

 +L

L

% B 

 + 

+L

Te m

pe ra

tu re

Liquid (L)

Temperature 

Pr es

su re

Solid (S)

Gas (G) Sublimation curve

Boiling curve

Melting curve

P-T diagrams T-x diagrams

PHASE DIAGRAMS AS YOUR’RE PROBABLY USED

TO SEEING THEM

• 712

Temperature

Composition

Pressure

A

B

G

S L

G

L

NOT AT ALL TO SCALE

Temperature

• Typical Binary Phase Diagrams

713

A B

+L L

% B  A B

 +L

L

% B 

 + 

+L

A B

+L

L

% B 

  +   + 

A B

+L

L

% B 

+ + 

 + 

Continuous Solid Solution: • Complete mixing of

components. • Components have same

crystal structure.

Primary (terminal) Solid Solution:

• Partial solubility of components.

• Hume Rothery rules apply.

Intermediate Solid Solution: • Almost always has a different

crystal structure than the phases on either side.

Intermediate Compound: • Almost always has a different

crystal structure than the phases on either side.

Two Phase Equilibrium

• Types of Systems/Reactions • Isomorphous

– Constituents are mutually soluble in all proportions and in all states.

• Eutectic – L  S1 + S2

• Eutectoid – S1  S2 + S3

• Peritectic – L + S1  S2

• Peritectoid – S1 + S2  S3

• Monotectic – L1  S + L2

• Syntectic – L1 + L2  S

714

Most phase diagrams are very complex.

Most include many of these reactions.

THIS IS WHY MATERIALS

SCIENCE IS SO COMPLICATED AND

FUN!

This is also why we get good jobs.

• Typical Ternary Phase Diagram

716 The same rules apply for ternary and higher order systems.

A, B, C = pure constituents

Sides = compositions of binary alloys and/or compounds.

y, z = compositions of ternary alloys and/or compounds.

y = alloy composed of 3 phases, p, q, and r.

z = alloy composed of 2 phases, m and n.

• 718

• 719

Fig. 11.27 Three isothermal sections for the ternary diagram shown in Fig. 11.26. A few of the tie lines are shown by dotted lines. (a) at a temperature below A-B eutectic temperature but above eutectic temperatures of the ternary, A-C and B-C; (b) at a temperature below the three binary eutectics but above the ternary eutectic, and (c) at a temperature below the ternary eutectic temperature. Adapted from Abbaschian, Reed-Hill, and Abbaschian, © 2009. Cengage Learning, Engineering. All Rights Reserved.

• 720

What is the composition at a given point?

Composition at point z:

• %A = XzA, %B =XzB, %C = XzC

XzA

XzB

XzCz

• 721

What is the composition at a given point (alternate way)?

What’s the composition at point z:

• %A = 100a/(a+b+c)

• %B = 100b/(a+b+c)

• %C = 100c/(a+b+c) b

c

a z

Lever Rule* Point z

% m = 100(zn)/(mn)

% n = 100(mz)/(mn)

Point y

% s = 100(yq)/(sq)

% q = 100(sy)/(sq)

* gives amounts

• Computed 1100°C Al-Ni-Pt isothermal section. V. Raghavan, Journal of Phase Equilibria and Diffusion, in press, 2010.

• 723

Figure 2

Phase diagram and lattice constants of a hypothetical alloy system. Adapted from Cullity and Stock, Elements of X-ray Diffraction, 3rd Edition (Prentice Hall, Upper Saddle River, NJ) p. 334.

Lattice parameters change when composition

changes.

A BPercent B 

1 2 3 4 5 6 7 8

Te m

pe ra

tu re

 Liquid

α (fcc)

β (fcc)

γ (bcc)

α + γ γ + β

γ + L

γ + L

α

β

a1 a3

a2 a4

x A BPercent B 

y

La tti

ce Pa

ra m

et er

s

• 724

In this system there are two terminal solid

solutions

α and β

There is one intermediate phase

γ

which is a line compound

A BPercent B 

1 2 3 4 5 6 7 8

Te m

pe ra

tu re

 Liquid

α (fcc)

β (fcc)

γ (bcc)

α + γ γ + β

γ + L

γ + L

α

β

a1 a3

a2 a4

x A BPercent B 

y

La tti

ce Pa

ra m

et er

s

Figure 2

Phase diagram and lattice constants of a hypothetical alloy system. Adapted from

Cullity and Stock, Elements of X-ray Diffraction, 3rd Edition (Prentice Hall, Upper

• Implications of solid solubility

• Solutes often expand or contract the crystal lattice.

725

Lattice expansion  in avg. a.

Lattice contraction  in avg. a.

• A BPercent B 

1 2 3 4 5 6 7 8

Te m

pe ra

tu re

Liquid

α (fcc)

β (fcc)

γ (bcc)

α + γ γ + β

γ + L

γ + Lα + L

β + L

α

β

a1 a3

a2 a4

x A BPercent B 

y

La tti

ce Pa

ra m

et er

s

726

What happens to your XRD pattern?

Figure 3: Calculated powder diffraction patterns for alloys 1 to 8 in the alloys system presented in Figure 2. Adapted from Cullity and Stock, Elements of X-ray Diffraction, 3rd Edition

(Prentice Hall, Upper Saddle River, NJ) p. 335.

The colored lines represent the relative locations of the XRD peaks for each phase

Increasing 2θ2θ = 0° 2θ = 180°

1

2

3

4

5

6

7

8

Increasing 2θ

• Key thing about XRD patterns

• Each phase has its own distinct XRD pattern which is just like a fingerprint for the phase.

• Peak locations for each phase in an XRD pattern are based upon unit cell dimensions.

• Thus each pattern will depend upon composition.

727

• Summary of results for phase diagram 1. Pattern for pure A. FCC crystal structure. Calculated lattice parameter

aA. 2. Pattern of -phase. Solid solution of A and B. In terms of atomic size

aB > aA. Lattice expands. Thus a increases up to the solubility limit. 3. Beyond  phase boundary. Precipitation of -phase. Superimposed

XRD patterns. Solubility of A in B does not change. Thus, lattice parameter of -phase does not change. Peak locations for -phase do not change.

4. Same pattern as (3). Only difference will be change in peak intensities (peak heights). This is due to a variation in the amounts of the -phase and -phase that are present. Remember the lever rule?

5. Only pure -phase is present. BCC crystal structure. Distinct from other patterns.

6. Superimposed patterns of -phase and -phase. The -phase is solid solution of A in B. aB < aA. Lattice contracts as more A is added to B.

7. Pattern of pure -phase. FCC crystal structure. Lattice parameter of  is greater than it was in (6) because there is less A in solid solution.

Recommended